Investigation of Mechanical and Thermal Properties on Novel Wheat Straw and PAN Fibre Hybrid Green Composites

Grewia optiva wheat straw waste fibre and PAN fibre are combined in this study to create new composite materials. The novel specimens were created in the hydraulic hind moulding machine with varying percentages of mass of wheat straw fibres, PAN fibre (2–8%) in an equivalent ratio with other materials, and Kevlar fibre-based composites (2–4%). Natural fibre-reinforced clothing is getting increasingly fashionable these days; thus, this research is important. In several papers, natural fibre has been stated to have the potential to replace synthetic fibres. Natural fibre reinforcing has also proven to be quite effective as composites. It is currently used in a range of fields, including medical fields, aerospace, and the automobile industry, among others. Synthetic fibres are used. The usage of synthetic fibres such as asbestos and Kevlar has already been linked to mesothelioma, a kind of lung cancer. Many people have died as a result of Kevlar and asbestos. As a result, an effort to replace these materials is ongoing. Fabricated material’s mechanical, chemical, physical, tribological, and thermal properties were evaluated.


Introduction
Because handling wheat-based waste bre has become a severe concern for India and the rest of the world, and these materials also pollute the environment, wheat bre waste material is being used [1]. ese compounds have been linked to major rail and highway safety concerns. On the other hand, this wastage is related to natural bres, and researchers are working on eco-friendly composites because Humans have used natural bres for thousands of years [2].
Because of their excellent qualities, natural bres are increasingly used to produce novel composites [3]. Recent synthetic bres have been investigated and found to have several environmental issues [4]. According to prior examinations and studies, asbestos and Kevlar, which are utilised in various applications, have been linked to the deaths of far too many people [5]. Asbestos and Kevlar were rst utilised because of their exceptional physical, mechanical, and chemical properties. Still, additional research has discovered that they cause a range of malignancies and major respiratory difficulties [6]. e World Health Organization (WHO) has placed restrictions on using asbestos after discovering its harmful effects [7]. e disadvantages are the low recycling rate, high cost, and environmental toxicity of this reinforced material. Kevlar has been shown in numerous studies to have a significant harmful influence on human health [8]. Ivy gourd is a fast-growing perennial plant native to tropical East Africa and South Asia and is broadly cultivated for its vegetable and medicinal uses in India. Coccinia grand is this plant's botanical name and is associated with the Cucurbitaceae family. is plant is an energetic creeper and grows to a height of 28 m. It starts flowering after two months of planting and is ready for harvesting after three months. On the other hand, natural fibres are light and easy to shape, less expensive, environmentally friendly, and biodegradable. It also has good tensile strength and a high specific strength [9]. Natural fibres are employed in a variety of applications these days, including plastering, building, construction, and transportation. [10]. It offers several advantages but also disadvantages, such as a higher moisture absorption rate. According to various sources, chemical treatments can change surface characteristics like porosity, tension, wetting, and adhesion strength. Few researchers stated that recent advances in manufacturing instruments, materials, and related technologies are solving the main challenges for deploying Class-II composite resin restorations. It is used in medical applications like dental care. To use the composites inside the human body, developing an innovative matrix system with simplified material for bulk-fill composites is essential. e collected bark fibres were submerged in water to induce microbial degradation for ten days, and a metal teeth brush was used for combing to extract quality fibres. Chemical functional groups were identified through FTIR analysis ranging from 4000 cm −1 to 500 cm −1 . OH stretching was observed at the peak of 3287 cm −1 . C-OH stretching was identified at the peak of 1013 cm −1 . e average surface roughness of the fibre was estimated at 4.88 nm through the Park XE 70 model atomic force microscope. Wheat is a major part of our crops and is grown worldwide. But thousands of tonnes of wheat waste fibre are also produced along with its cause, which is very difficult to handle and produces many kinds of pollution [10]. Many researchers stated that epoxy resin is significantly used as a matrix material in various aerospace, shipbuilding, automobile industry, and structural applications. e epoxy and glass fibre is mixed in a ratio of 1 : 1 to obtain the best mechanical properties.
A novel of this research aims to develop a green composite utilised wheat fibre. e mechanical qualities of PAN fibre are utilised in hot gas filtration systems, concrete strengthening, sweater and socks manufacture, and other applications. Despite the fact that PAN has excellent frictional properties, natural fibres have been used as reinforcement materials. Wheat straw and PAN fibres have also been used as reinforcement materials with good results.

Materials and Composite Fabrication.
Wheat straw fibres were gathered from Ghanotala village in Hamirpur, India. e wheat straw fibre was cut into small pieces and soaked in water for four weeks. Afterwards, the fibre was rinsed in deionized water and dried for two days. To remove any potential contaminants, the recovered fibre was soaked in sodium hydroxide (Noah) for 24 hours [11]. e fibre was chopped for 15 minutes. e natural and PAN fibres were then joined with other elements utilised in the construction of new composite materials (phenolic resin, barium sulphate (BaSO 4 ), potassium titan, ceramic, and mica) [12]. Tables 1 and 2 demonstrate the technique.

Characterization of Physical-Mechanical and ermal
Properties.
e impact test was carried out using a pendulum impact testing machine. e test sample was immersed in oil for two days to measure porosity [13]. A Glun Digital measuring scale was used to determine density. By immersing new samples in water for one day, the standard (ASTMD570-98) was utilised to determine their water absorption [14]. Mechanical parameters were determined using universal testing equipment.

Testing of Tri-Biological Characteristics of Developed
Composites.
e tribological properties of samples were tested on a chase machine especially utilised to find the characteristics at different temperatures. e new samples were tested to find wear, recovery, stability, fade, and variability [16]. e load was taken at 700 N, and the temperature maintained for 100-300°C reading was taken after each 50°C interval [17]. Figure 1 shows the compressive strength and Shear strength of newly developed composites. e compressive strength of 2% based composites was determined to be the highest for wheat straw-PAN and Kevlarbased composites, while WF-4 (8%) and FK-2 (4%) composites have shown their lowest value. e shear strength has the maximum value for wheat straw-PAN-based composites for WH-2 (4%]) and also shows its strength for WH-4-based composites [18]. As the wheat-PAN fibre heat at low temperature, they expand and heat swelling increases. e tensile strength was observed highest at 4% based on wheat-PAN fibre composites and also showed minimum strength for WH-1. e Kevlar-based composites showed the highest tensile and shear strength values for FK-1 composites [19]. As the wheat-PAN and Kevlar increase in the matrix, the compressibility increases [20]. Compressibility was highest for WF-4 and FK-2 composites, while it was lowest for 2% wheat straw and Kevlar-based composites, as illustrated in Figure 2 [21]. e inclusion of wheat straw-PAN and Kevlar in the newly created samples increased porosity because wheat-PAN and Kevlar (light wt.) have taken the place of barium sulphate heavy materials [22]. WH-4 and FK-2 have shown maximum heat swelling [23]. Each test has been repeated three times, and average values have been taken. e standard deviation is 0.25 observed during the experiments. Figure 3 shows the porosity and heat swelling of newly developed composites [24]. e density of wheat-PAN and Kevlar-based composites decreases with an increased percentage in polymer matrix compared to porosity [25]. e porosity and density are directly related to other properties    like water absorption and compressibility [26]. Figure 4 shows the density and hardness of newly developed composites [27]. At high density and low porosity, the water absorption will be low, compressibility will be low, and opposite to it, low at density and high porosity, the water absorption will be high compressibility [28]. Figure 4 shows    International Journal of Chemical Engineering that hardness was at its highest for WF-1 and FK-1-based composites, while it was at its lowest for WF-4 and FK-2based specimens [29]. Figure 5 shows that WF-4 and FK-2based composites have the highest water absorption, while WF-1 and FK-1 composites have better outcomes [30]. e ash percentage was highest for WF-1 and F-1-based composites as shown in Figure 5. Figure 6 shows that the impact energy was highest for WF-1 and FK-1 composites. e failure strain was highest at WF-1 and FK-1 while proof stress was highest at WF-2 and FK-2 as shown in Figure 6 [31]. e fibre's rough surface and morphological properties are important to achieve better interfacial bonding in composites, which decides the composites' load-bearing capacity and performance [32]. ey identified the flaky honeycomb and rough surface morphology of Cissus quadrangularis root fibre through the scanning electron microscope [33].

Fade and Recovery Performance Analysis.
e fade percentage of new specimens has increased as increased the percentage of wheat straw fibre-PAN in the new composition (2% � 35.7, 4% � 37.4, 6% � 39.2, and 8% � 40.5), while the increased percentage of Kevlar in the new composition has also increased the fade percentage (2% 34.5 and 4% � 36.3) [34]. As indicated in Figure 7, recovery rose as the percentage of Kevlar (2% � 110.3, 4% � 108.5) and wheat straw fibre (2% � 101%, 4% � 103%, 6% � 107%, and 8% � 108) increased [35]. Organic fibre generates a heterogeneous matrix and shears quickly, acting as third-body particles [36]. is explains why a higher proportion of wheat straw fibre-PAN in the polymer composite causes more fade and wear [37]. Figure 8 illustrates the wear range for wheat straw fibre-PAN composites, which is between 1.3 and 1.6 g, while for Kevlar-based polymer composites, it is between 1.25 and 1.3 g [38]. According to the wear test, increasing the proportion of wheat straw fibre-PAN and Kevlar in composites improves the wear rate. e WF-1 composite had the least wear, while the GF-4 composite had the greatest [39]. ey made samples with a higher percentage of wheat straw fibre-PAN and Kevlar fibre, which has not shown a homogenous matrix well with the other polymer composite components and causes the wear rate to increase [40]. FK-1 composites are less worn than FK-2 composites. e triple-layer hybrid composites use almond and kenaf fibres with epoxy resin as a matrix [41]. Two kinds of triple layer composites were fabricated using the hand lay-up method, where fibres are laid in order as kenaf/almond/ kenaf and almond/kenaf/almond. Test results show the high tensile (85 MPa) and flexural (92 MPa) properties for the kenaf/almond/kenaf layer composite [42].
is flaky rough surface of the fibres contributes to better mechanical properties while making it a composite due to the increased bonding feature of the fibre with the matrix [45]. Moreover, the thermal behaviour of Cissus quadrangularis root fibre was studied using Jupiter simultaneous thermo gravimetric analyser (Model STA 449 F3, Netzsch, International Journal of Chemical Engineering 5 Germany) from 28°C to 1000°C in a nitrogen atmosphere with a 20 ml/min rate of flow and heating at 10°C/min [45].

TGA of Wheat Straw Fibre-PAN-Based Samples and
Kevlar-Based Samples. e TGA test of freshly produced experiments was carried out in a nitrogen [N2] atmosphere, as shown in Figure 10 [46]. e best thermal stability was discovered in WF-4 [47]. In Kevlar-based composites, FK-2 offers better thermal stability in this test. During the test, it was determined that there were three zones of degradation [48].
e first zone showed minimal degradation due to water particles in the composite's significant degradation between 250°and 600°C [49]. In contrast, the second zone showed significant degradation between 250°and 600°C, which could be due to a decrease in hydrogen bonding in Kevlar composites, as well as hemicellulose loss and gas release from wheat straw fiber-PAN composites [50]. e third drop was found in the temperature ranges of 600°C and 800°C. ere was relatively minimal degradation in the created samples [51]. e loss of lignin and cellulose from Kevlar and the removal of the amide group. e third degradation is caused by the removal of the amide group and the loss of lignin and cellulose from Kevlar and wheat straw fibre-PAN [52].

Conclusions
After all physical-chemical, mechanical, tribological, and thermal testing were completed, the following results were evaluated: Wheat straw-PAN composites had the best recovery percentage at 8% composition. In contrast, 4% composition of Kevlar-based composites has shown maximum recovery. Composites with 2% wheat waste fibre-PAN and Kevlar-based fibres had the lowest fade percentage. e lowest variability and best stability coefficients were found in all of the newly produced samples (stability). WF-1 (2%) and FK-1 (2%) equals FK-1 (2%) (2%) and FK-1 (2%) composition-based composites were found to have the least amount of heat swelling. In terms of wear, WH-1 (2%) and FK-1 (2%) have shown a minimum wear rate. In composites containing 2% wheat-PAN fibres, water absorption, porosity, and compressibility were found to be low. e composites based on WH-1 were found to have the highest hardness. Shear strength was found to be highest in WF-2 (4%) and FK-1 (2%), while tensile strength was highest in WF-2 (4%). e WF-1 (2%) and FK-1 (2%) composites had the maximum compressive strength and impact energy. Wheat-PAN fiber offers the maximum thermal stability for WH-4. WF-1 has given excellent results in maximum characterization.

Data Availability
e data used to support the findings of this study are included in the article. Should further data or information be required, these are available from the corresponding author upon request.

Conflicts of Interest
e authors declare that there are no conflicts of interest regarding the publication of this paper.  International Journal of Chemical Engineering